A. Bozzi et al. / Journal of Photochemistry and Photobiology A: Chemistry 174 (2005) 156–164 157water ; (b) at 100 ◦ C from sol–gel exposed to water vapor talline and amorphous regions. The C2 and E cotton samples; (c) at temperatures 60–180 ◦ C from TiO2 –SiO2 ﬁlms ex- were pretreated in a conventional RF-plasma cavity (Har-posed to water vapor . In the last case, the treatment with rick and Co., UK). A variety of functional groups like: C O,water vapor reduced the temperature necessary to produce O C O, COH, COOH, CH2 OH were introduced onanatase crystallites in the sol–gel ﬁlms to temperatures be- the fabric surface through the reaction between the active O-low 100 ◦ C by phase separation of the TiO2 from the SiO2 ; species (singlet 1 O2 , atomic O, anion-radical O− and cation-(d) anatase nano-crystals were produced more recently on radical O+ ) induced by the plasma activation of the gas phasecotton fabrics from the TTIP alkoxide solution at low tem- on the carbon textile surface . These oxygen function-perature by sol–gel process with grain sizes of ∼20 nm. The alities obtained in the 0.1 mbar cavity of the RF-plasma at-anatase phase was attained on the cotton textile surface by tained a higher concentration with longer treatment times upboiling the textiles in water for 3 h . to ∼30 min. This time has been chosen for RF-plasma pre- Acrylic emulsions of TiO2 have been coated on tex- treatment during this study. Recently, the preparation of di-tiles with the purpose of inducing self-cleaning effects un- verse catalysts using plasma technology has been describedder daylight irradiation , but the coating showed some [17,18]. The experimental conditions used during the RF-degradation after being exposed to the action of daylight. plasma pretreatment were: plasma generator at 13.56 MHz;Another low temperature ﬁxation of TiO2 anatase nano- plasma power 100 W and a residual gas pressure of 0.1 mbar.crystals on plastic substrates has been carried out recentlyfrom silica–titania gels showing anatase cluster formation 2.2.2. MW-plasmaafter hot water treatment . The direct preparation of The C2 and E cotton samples were also pretreated in aanatase/polymer nano-composite ﬁlms from sol–gel titania MW-plasma cavity (Vacotec Corp., Neuchatel, Switzerland).on polymer ﬁlms is generally not possible due to the low re- A schematic representation of the MW-plasma unit is shownsistance of the organic polymers to heat treatment [14,15]. in Fig. 1. Experiments were performed at 2.45 GHz. TheRecently polymers ﬁlms with negative surface groups have power was varied from 100 to 600 W, the reaction times werebeen exchanged with TiO2 to attach the titania on their surface changed from 10 to 180 s, the gas ﬂow was between 20 andby electrostatic attraction . One of the reasons to under- 100 ml/min, and the gas pressure varied from 0.02 to 2 mbar.take the present research is to explore the commercial poten- Before the sample treatments the plasma MW-chamber wastial of the TiO2 semiconductor on cotton textiles prepared at evacuated for 2 h up to 0.01 mbar. MW-plasma in air (air-relatively low temperatures for self-cleaning purposes. This MW-Plasma) was used to oxidize the cotton surface. Thestudy aims at the discoloration of organic materials includ- pretreatment time was varied between 5 and 45 s and usu-ing dyes, pigments and grease on the modiﬁed cotton textile ally 120 ◦ C were not exceeded in this way. This is belowloaded with TiO2 . The use of TiO2 loaded ﬂexible substrates the temperature of 180 ◦ C the upper limit for cotton textiles.will possibly allow their application during the photodegrada- The ionized gas is composed atomic oxygen, ionic forms oftion of micelles, oils, solvents, sooth, aromatic and aliphatic oxygen (negative and positive), radicals formed due to thehydrocarbons under daylight. interaction of O-excited species and residual water vapor. 2.2.3. Vacuum–UV (V–UV)2. Experimental The cotton fabrics were also pretreated using the 185 nm line of a low pressure mercury source from Ebara Corp.,2.1. Materials Iwasaki Electric Co., Shiba, Japan having a power of 25 W. The scheme of the installation used is shown in Fig. 2. The Base treated cotton (C2 ) and mercerized cotton samples lamp wall consists of synthetic silica able to transmit the(E) were used throughout this work. The mercerized cot-ton network contained a variety of stabilizers, oxidants andtensides to eliminate the natural grease, pectine, lignine andstains associated with untreated cotton ﬁbers. Titanium tetra-chloride (TiCl4 ), titanium tetra-isopropoxide (TTIP), nitricacid (HNO3 ) and hydrochloric acid (HCl) were Fluka p.a.reagents and used as received. Triple distilled water was usedin all experiments.2.2. Pretreatment of synthetic textiles fabrics2.2.1. RF-plasma Cellulose is the main component of wood and plant ﬁbers.Cotton is almost pure cellulose formed by d-glucose units Fig. 1. Schematic of a microwave-plasma (MW-plasma) unit used to pretreatand its macro-structure is heterogeneous consisting of crys- the surface of cotton textiles.
158 A. Bozzi et al. / Journal of Photochemistry and Photobiology A: Chemistry 174 (2005) 156–164 Fig. 2. Schematic of the V–UV unit used to pretreat the surface of cotton textiles.184 nm lights. This wavelength comprises 25% of the total and peroxide groups form upon either pretreatment . Thelamp output. 75% of the lamp output consisted of 254 nm bac- overall hydrophilicity of the textile surface was observed totericide radiation. Since the vacuum–UV activation proceeds drastically increase due to this pretreatment.with a lower energy than the plasma activation, no cationicor anionic oxygen species are formed in the gas phase. Only 2.3. Preparation of TiO2 colloidsatomic and excited oxygen species are formed and this isthe difference with the plasma methods described in section 2.3.1. TTIP as colloidal TiO2 precursor(a) and (b) above. This leads to a more deﬁned and uniform Titanium tetra-isopropoxide (TTIP, 20 ml) was addedmodiﬁcation of the textile surfaces with an increased polar- drop-wise to 300 ml of 2-propanol acidiﬁed by 1 ml of con-ity because it contains a variety of oxygen functional groups centrated HNO3 and cooled at ∼0 ◦ C in an ice bath. The solu-formed by the reactions of free radicals with the O2 in the tion was stirred for ∼1 h to attain total dissolution of the poly-gas phase. The upper textile layers are excited by the incom- meric chains and produce a transparent colloidal solution.ing UV light up to ∼100 A or the equivalent of about 50 ˚atomic layers [17,18]. Either by plasma or by vacuum–UV 2.3.2. TiCl4 as colloidal TiO2 precursorpretreatment the residual oxygen at the pressures worked was An aliquot of 10 ml TiCl4 were slowly added to 1 L (0.5 Msufﬁcient to modify the textile surfaces due to the absorption HCl) aqueous solution. The reaction vessel was immersed incross-section of the O2 for plasma radiation or ultraviolet an ice-bath to prevent precipitation of TiO2 polymeric-sollight. Fig. 3 shows in a simpliﬁed way the functional groups during to the kinetically fast and highly exothermic hydrol-introduced in the cotton ﬁbers by plasma or V–UV treatment. ysis process. The Cl− -ions in the solution were eliminatedA signiﬁcant number of carboxylic, percarboxylic, epoxide by dialysis adding continuously distilled water within 2 days Fig. 3. Diagram indicating the modiﬁcation of cotton textiles induced by plasma or V–UV pretreatment.
A. Bozzi et al. / Journal of Photochemistry and Photobiology A: Chemistry 174 (2005) 156–164 159using a cellulose membrane. The Cl− -ions have to be elimi- was measured in a GC (Carlo Erba, Milano) provided with anated since they interfere during the photo-catalytic destruc- Poropak S column.tion of the stains by the TiO2 clusters on the textile surface. 2.6. Elemental analysis Elemental analysis of the TiO2 loading on the textile fab-2.4. Deposition of colloidal and TiO2 Degussa P25 rics was carried out by atomic absorption spectrometry usingpowder coated textiles a Perkin-Elmer 300 S unit.2.4.1. Colloidal TiO2 2.7. Transmission electron microscopy (TEM) Pretreated 4 × 12 cm textiles samples were immersed inthe chosen TiO2 colloidal suspension and exchanged for A Philips CM 300 (ﬁeld emission gun, 300 kV, 0.17 nm30 min as described in Section 2.2. Afterwards, the samples resolution) HRTEM microscope and a Philips EM 430were dried in two steps: (a) ﬁrst in air for 24 h at 22 ◦ C (lab- (300 kV, LaB6 , 0.23 nm resolution), provided with energyoratory temperature) and (b) followed by heating at 100 ◦ C dispersive spectrometers (EDS) were used to measure thefor 15 min. The exchange operation to load the TiO2 on the particles sizes of the titania clusters coating the textile fab-textiles was carried out immediately after the fabric pretreat- rics. The textiles were embedded in epoxy resin (Embed 812)ment by any of the three techniques mentioned above. The and the fabrics were cross-sectioned with an ultra-microtomereason for this is that the radicals formed at the fabric surface (Ultracut E, Reichert-Jung) to a thin section of 50–70 nm.react with the humidity and oxygen of the air. This deacti- Magniﬁcation from about 1000× to 450,000× were used tovates the radicals induced by the pretreatment. The textile characterize the samples and this allowed the determinationsamples were then washed with distilled water under son- of the TiO2 cluster size up to the nanometer range.ication to remove the TiO2 particles that did not attach tothe fabric surface. During this study we found that only pre- 2.8. X-ray diffractiontreated surfaces were able to ﬁx TiO2 from colloidal solutions(or powder suspensions or the combination of both. The dyes The crystallographic phase of the TiO2 on the textile sam-with carboxylate groups have been recently reported to be ples was determined by a Siemens X-ray diffractometer usingable to anchor TiO2 via coordination . Cu K␣ radiation.2.4.2. TiO2 Degussa P25 powder 3. Results and discussion The pretreated cotton textiles were immersed in a previ-ously sonicated (30 min) aqueous solution of TiO2 Degussa 3.1. Development of CO2 due to the degradation ofP25 (5 g/l) and heated for 1 h at 75 ◦ C. The textile was dried wine, coffee, make-up and grease stains on C2 and Efor 1 h at 100 ◦ C and then the unattached TiO2 particles on cotton textiles prepared by different methodsthe textile surface were washed out in distilled water by 5 minsonication. A loading of 1.0–1.5% (w/w) for the sample 7 of Table 1 shows the values of the CO2 volumes formed dur-Table 3 was determined by elemental analysis (see Section ing mineralization of organic various stains by TiO2 under2.6). light. In practice besides the CO2 a small amount of inor- ganic anions and cations are also produced during the min-2.5. Irradiation procedure and evaluation of the textiles eralization process since the chromophore functional groupscleaning action of red wine contain lycopenes, carotenoids and other natural pigments besides a small amount of cations and anions. The The photochemical reactor consisted of 80 ml cylindrical reaction vessel described in Section 2.5 of the experimentalPyrex ﬂasks containing a strip of textile of 48 cm2 positioned part was used for the CO2 determination. The evolution ofimmediately behind the wall of the reactor. The wine stains CO2 of a red wine stain on C2 cotton pretreated by RF-plasmaare introduced on the cotton fabric using a micro-syringe with after 24 h irradiation is shown in the ﬁrst line of Table 1 to50 l of red wine. The irradiation of samples was carried out produce the highest amount of CO2 (2000 l) under solarin the cavity of a Suntest solar simulator (Hanau, Germany) simulated light (50 mW/cm2 ).air-cooled at 45 ◦ C. The Suntest lamp had a wavelength distri- Fig. 4 shows the evolution of CO2 as a function of irradi-bution with 7% of the photons between 290 and 400 nm. The ation time for wine stains. It is seen that the CO2 evolutionproﬁle of the photons emitted between 400 and 800 nm fol- increases at a slower pace at the beginning and more steeplylowed the solar spectrum with a light intensity of 50 mW/cm2 above 8 h irradiation (trace c). Very small amounts of CO2corresponding to 50% of AM1 (AM1 is light intensity of the were observed when cotton was irradiated with daylight inmidday equatorial solar radiation). The radiant ﬂux was mon- the absence of TiO2 and wine (trace a). Also, small amountsitored by a LSI Corporation power meter of Yellow Springs, of CO2 were observed when the cotton was stained with wineCO., USA. The CO2 volume produced during the irradiation in the absence of TiO2 (trace b).
160 A. Bozzi et al. / Journal of Photochemistry and Photobiology A: Chemistry 174 (2005) 156–164Table 1Textile type C2Sample name Pre-treatment Pre-treatment time TiO2 precursor Red wine spot Coffee spot Make-up-spot Grease spot CO2 (l) CO2 (l) CO2 (l) CO2 (l)C2–2 RF-plasma 60 min TiCl4 2000 1800 1350 1900C2–3 V–UV 15 min TTIP 1700 1430 1050 1270C2–4 V–UV 30 min TTIP 1000 960 680 860C2–5 V–UV 15 min TiCL4 1800 1280 880 1010C2–6 V–UV 60 min TTIP 700 700 530 710C2–13 MW-plasma 15 s TTIP 1200 1150 550 540C2–14 MW-plasma 30 s TTIP 1200 1830 890 1330C2–15 MW-plasma 15 s TiCl4 600 690 720 620C2–16 MW-plasma 30 s TiCl4 600 790 400 290 TTIP sol–gel having a favorable action on the TiO2 structure and dispersion on the textile surface. Generally the amount of CO2 evolved under Suntest light irradiation on cotton (C2 ) is signiﬁcantly higher than for the mercerized cotton (E) sam- ples. This is due to the adverse effect of the networking, sur- face and oxidative additives used to mercerize the cotton (E) samples. The TiO2 loaded textile allows for bigger time inter- vals for the cleaning by conventional methods since the red wine stains are already partially degraded on the TiO2 loaded textiles due to the action of daylight and will be more recep- tive towards the application of detergents during household washing with the accompanying cost saving. Table 3 shows the discoloration of red wine stains pre- pared from different procedures on the cotton sample (C2 ) but pretreating with the UV-irradiation unit shown in Fig. 3. By inspection of Table 3 it is seen that the surface textiles pre-Fig. 4. CO2 evolution under Suntest light irradiation (50 mW/cm2 equivalentto the daylight intensity in Switzerland in an average day) for C2 cotton treated with two UV low-pressure mercury lamps evolved thesamples pretreated for 30 min by V–UV as a function of time: (a) cotton highest quantity of CO2 from red wine stains. These quanti-C2 alone; (b) cotton C2 with wine stain; and (c) cotton sample C2-2 stained ties are 5–7 times higher in l CO2 compared to the to CO2with wine. evolved by red wine stains on textiles not coated with TiO2 (see Table 1) for textiles pretreated with only one UV lamp. Table 2 presents the results for the evolution of CO2 from The results shown in Table 3 use the reactor shown in Fig. 3the discoloring and/or decomposition of the wine stain on to perform the experiments allowing for a better geometrymercerized cotton samples (E). The sample E-19 with a red and a closer distance between the cotton sample and the lightwine stain shows the most favorable CO2 evolution after 24 h source. The TiO2 Degussa P25 powder loading of the cot-Suntest light irradiation. It was prepared using TTIP as the ton sample consisting of 80% anatase and 20% rutile havingTiO2 precursor and pretreating with MW-plasma for 15 s. The crystalline sizes of 30–40 nm seems to be the most suitableMW-plasma treatment that is accompanied by heat seems to titania active in the removal of the pigments associated withincrease the contact between the cotton tissue and the surface red wine stains.Table 2Textile type ESamples name Pre-treatment Pre-treatment time TiO2 precursor Red wine spot Coffee spot Make-up spot Grease spot CO2 (nl) CO2 (nl) CO2 (Hi) CO2 (nl)E-7 RF-plasma 60 min TTIP 200 300 250 360E-8 RF-plasma 60 min TiCl4 125 160 150 150E-9 V–UV 15 min TTIP 150 150 140 190E-10 V–UV 30 min TTIP 140 170 130 120E-11 V–UV 15 min TiCl4 100 130 160 190E-12 V–UV 60 min TiCl4 160 220 150 160E-17 MW-plasma 15 s TiCl4 550 450 370 460E-18 MW-plasma 30 s TiCl4 170 250 330 280E-19 MW-plasma 15 s TTIP 700 800 690 620E-20 MW-plasma 30 s TTIP 600 650 610 640
A. Bozzi et al. / Journal of Photochemistry and Photobiology A: Chemistry 174 (2005) 156–164 161Table 3UV pretreated cotton type C2 red wine stainsSample name Gas Lighted lamps TiO2 source Stain CO2 after 24 h irradiation (area)Sample 7 Air 2 lamps Degussa P25 Wine 11807Sample 14 Argon 8 lamps TiO2 (TTIP 10–15 nm) Wine 11501Sample 13 Argon 8 lamps Degussa P25 Wine 11112Sample 10 Air 8 lamps TiO2 (TTIP 10–15 nm) Wine 11064Sample 3 Vacuum 2 lamps Degussa P25 Wine 9783Sample 6 Vacuum 8 lamps TiO2 (TTIP 10–15 nm) Wine 9724Sample 11 Argon 2 lamps Degussa P25 Wine 9391Sample 5 Vacuum 8 lamps Degussa P25 Wine 8986Sample 9 Air 8 lamps Degussa P25 Wine 8792Sample 12 Argon 4 lamps Degussa P25 Wine 7659Sample 4 Vacuum 4 lamps Degussa P25 Wine 7407Sample 8 Air 4 lamps Degussa P25 Wine 7003Table 4UV pretreated cotton type C2 coffee stainsSample name Gas Lighted lamps TiO2 source Stain CO2 after 24 h irradiation (area)Sample 7 Air 2 lamps Degussa P25 Coffee 12308Sample 14 Argon 8 lamps TiO2 (TTIP 10–15 nm) Coffee 11769Sample 13 Argon 8 lamps Degussa P25 Coffee 10192Sample 3 Vacuum 2 lamps Degussa P25 Coffee 9748Sample 10 Air 8 lamps TiO2 (TTIP 10–15 nm) Coffee 9407Sample 6 Vacuum 8 lamps TiO2 (TTIP 10–15 nm) Coffee 7682Sample 8 Air 4 lamps Degussa P25 Coffee 7578Sample 12 Argon 4 lamps Degussa P25 Coffee 7294Sample 5 Vacuum 8 lamps Degussa P25 Coffee 7224Sample 4 Vacuum 4 lamps Degussa P25 Coffee 6530Sample 9 Air 8 lamps Degussa P25 Coffee 6183Sample 11 Argon 2 lamps Degussa P25 Coffee 6132 Table 4 shows the discoloration of a coffee stain from only for the absorption of 4% of the incident light [1–4] adifferent TiO2 precursors on the cotton sample (C2 ) and pre- multilayer TiO2 coating would be favourable for the photo-treating with the UV unit shown in Fig. 3. By inspection of catalytic activity specially leading to increased or total TiO2Table 4, it is seen that the pretreated cotton with two UV low light absorption.pressure mercury lamps evolved the highest quantity of CO2from the coffee stains.3.2. Transmission electron microscopy of the mostefﬁcient samples used in red wine discoloration oncotton textiles Fig. 5 presents the cross section of one cotton ﬁbre on thesample C2-2 loaded with TiO2 after 20 household washings.The TiO2 layer was observed to be present in the same formas before the washing cycles. This lends support to the stableﬁxation achieved for TiO2 on the cotton C2-2 ﬁbres. Thissample has been described in Table 1. The TiO2 layer had athickness of 180–300 nm. The sample C2-2 shows the highestCO2 evolution from the decomposition of wine stains underdaylight irradiation. This is the reason why this sample wasselected to perform the TEM observation. These TEM resultsstrongly suggested that TiO2 crystalline clusters on the cot-ton surface accounts for only a small amount of the total areaof the textile covered by TiO2 . The titania on the textiles wasidentiﬁed by energy dispersive spectrometry (EDS) showingthat only a fraction of the TiO2 on the cotton was in a crys- Fig. 5. Transmission electron microscopy of a cotton textile sample C2-2talline phase. The multilayer TiO2 coating was prepared from showing the stable TiO2 coating after 20 washings. For other experimentalthe TiCl4 precursor. Since one monolayer of TiO2 accounts details see text.
162 A. Bozzi et al. / Journal of Photochemistry and Photobiology A: Chemistry 174 (2005) 156–164 Fig. 8. Classical scheme for the production of highly oxidative species by TiO2 under light irradiation with wavelengths <400 nm. is a conﬁrmation that a high dispersion of TiO2 clusters was attained on the E-cotton samples.Fig. 6. Transmission electron microscopy of a cotton textile sample E19 3.3. Mechanism suggested for the discoloration of stainsshowing the TiO2 coating around a single cotton ﬁber. For other experimental on cotton textilesdetails see text. Fig. 8 shows the accepted mechanism during the last 25 Fig. 6 shows the TiO2 coating around E-19 single cotton years for the generation of highly oxidative radicals on theﬁber loaded with TiO2 in the way described in Table 2. A TiO2 surface when light below 400 nm is applied on the pho-TiO2 coating of 150–220 nm thick was observed by TEM. tocatalyst surface [19,20]. Fig. 9a shows the intervention ofClusters of TiO2 between 5.77 and 6.80 nm were found by TiO2 under daylight irradiation when photo-decomposingHRTEM on the E-19 surface and are shown in Fig. 7. This a grease stain. The Suntest light which follows the solarFig. 7. High resolution transmission electron microscopy (HRTEM) of a Fig. 9. (a) Suggested scheme for the discoloration of grease stains undercotton textile sample E19 showing the TiO2 clusters before washing. This Suntest light irradiation mediated by TiO2 photocatalyis. (b) Suggestedﬁgure was Fourier ﬁltered to enhance the atomic lattice constant. For other scheme for the discoloration of wine and coffee stains under Suntest lightexperimental details see text. irradiation by TiO2 photocatalyis.
A. Bozzi et al. / Journal of Photochemistry and Photobiology A: Chemistry 174 (2005) 156–164 163Fig. 10. Mechanism of photo-discoloration of the tannin pigment of wineunder daylight irradiation.spectrum is absorbed directly by the TiO2 since the greaseabsorbs light only <290 nm. The mechanism of stains absorbing the incoming daylightradiation is shown in Fig. 9b. This is known from severalstudies during the last 20 years suggesting a dye sensitizedprocess when synthetic dyes like Orange are used [21,22].Fig. 9b presents the scheme for the discoloration of the natu- Fig. 11. (a) X-ray diffraction of (a) cotton C2-13 samples loaded with TTIPral colored pigment RH due to the generation of OH◦ , HO2 ◦ at time zero; (b) cotton C2-13 sample loaded with TTIP after 24 h irradiationand H2 O2 on the TiO2 surface . Fig. 9b suggests that in with Suntest solar simulated light (50 mW/cm2 ); and (c) cotton C2 blank. (b)the case of synthetic dyes colored pigments sensitize a pro- X-ray diffraction of cotton C2-2 samples loaded with TiCl4 after RF-plasmacess leading to dye discoloration under daylight irradiation. pretreatment after a 60 min photo-discoloration of a wine stain using Suntest irradiation. The peaks marked with a small arrow correspond to the positionThe decomposition of the organic compound goes through a of rutile peaks.cation intermediate (stain+ ) leading ultimately to the produc-tion of CO2 . The electron injected into the TiO2 conductionband starts the oxidative radical-chain leading to stain dis- wine stain. Fig. 11b shows the C2-2 sample before irradia-coloration. tion. The position of the rutile peaks is indicated by arrows Fig. 10 shows the mechanism for tannin photo-degradation in Fig. 11b. The sample C2-2, shows a high stain mineral-in analogy with the photo-induced degradation reported re- ization efﬁciency for red wine, coffee, make-up and greasecently for the lycopene, a natural pigment [24,25]. The tan- (Table 1) due to the presence of amorphous and rutile phasenins and lycopenes are pigments found in plants and fruits. TiO2 .Lycopene is a pigment of the carotenoid family. It is not onlyfound in the red wine used a probe molecule during this studybut it also gives its particular color to tomatoes and other veg- 4. Conclusionsetables. Cotton textiles of the type C2 were treated with ammonia3.4. X-ray diffraction studies of loaded TiO2 surfaces only mineralize more effectively stains of pigmented com- pounds and grease upon TiO2 loading under daylight than E- Fig. 11a shows the X-ray diffraction pattern for a blank cotton textiles containing several additives and surface form-C2 sample (trace c) and for the samples C2-13 (see Table 1 ing agents. When light is harvested directly by the TiO2 , anfor the preparation details). Traces (a) and (b) before and increased CO2 evolution was observed with respect to wineafter discoloration of a wine stain after 24 h with Suntest and coffee stains under similar experimental conditions onlight are also shown in Fig. 11a. No crystalline phases of the same TiO2 loaded textile. The surface pretreatment ofTiO2 were found in traces (b) and (c). It is interesting to note the cotton textile used in this study allows to attach TiO2that the cotton sample C2-13 loaded with amorphous TiO2 directly on the textile by functionalization of the cotton tex-as shown by trace (b) was able to discolor the wine stain tile with a variable density of functional groups negatively(Table 1). No difference is observed between traces (b) and charged. This pretreatment seems not to degrade the cotton(c) in Fig. 11 showing the stability of the amorphous TiO2 surface. The pretreatment is applied in dry conditions in thecoating on the cotton during the photo-degradation of the absence of solvents. Also, the times employed for the cotton
164 A. Bozzi et al. / Journal of Photochemistry and Photobiology A: Chemistry 174 (2005) 156–164surface modiﬁcation were short and involved reduced energy  M. Noorjahan, V.D. Kumari, M. Subrahmanyan, P. Boule, Appl.requirements. Catal. B 47 (2004) 209–213.  W.A. Daoud, J.H. Xin, J. Am. Ceram. Soc. 87 (2004) 953–955.  M. Noorjahan, V. Durga Kumari, M. Subrahmanyan, P. Boule, Appl. Catal. B 47 (2004) 209–213.Acknowledgments  A. Matsuda, T. Matoda, T. Kogure, K. Tadanaga, T. Minami, M. Tatsumisago, J. Sol–Gel Sci. Technol. 27 (2003) 61–69.  M. Dhananjeyan, E. Mielczarski, K. Thampi, Ph. Buffat, M. Bensi- This study was supported by KTI/CTI TOP-NANO 21 mon, A. Kulik, J. Mielczarski, J. Kiwi, J. Phys. Chem. B 105 (2001)program under Grant no. 6117.2 TNS (Bern, Switzerland) in 12046–12055.cooperation with AG Cilander, Herisau 9101, CH and COST  L. Xiao-e, A. Green, S. Haque, A. Mills, J. Durrant, J. Photochem.D19 under Grant no. C02.0068 (OFES, Bern, Switzerland). Photobiol. A 162 (2004) 253–259.  J.M. Grace, L. Gerenser, J. Dispersion Sci. Technol. 24 (2003) 305–341.  C.M. Chan, T.M. Ko, H. Hiroaka, Surf. Sci. Rep. 24 (1996) 1–54.References  Ch. Liu, G. Vissokov, B. Jang, Catal. Today 72 (2002) 173–184.  A. Nozik, Photo-Effects at the Semiconductor-Electrolyte Interfaces, A. Mills, S.K. Lee, J. Photochem. Photobiol. A 152 (2002) 233–247. ACS Symposium Series 146, Am. Chem. Soc., Washington, DC, A. Fujishima, T.N. Rao, D. Tryk, J. Photochem. Photobiol. C: Pho- 1981. tochem. Rev. 1 (2000) 21.  S.Roy Morrison, Electrochemistry at Semiconductor and Oxidized M. Langlet, A. Kim, M. Audier, J.-M. Herrmann, J. Sol–Gel Sci. Metal Electrodes, Plenum Press, New York, 1982. Technol. 25 (2002) 223–234.  J. Kiwi, in: A. Harriman, M.A. West (Eds.), Photodegradation of Th. Oppenlaender, Photochemical Puriﬁcation of Water and Air, Hydrogen, Academic Press, London, 1982, pp. 119–145. Wiley-VCH, Winheim, Germany, 2003.  D. Adams, L. Brus, C. Chidsey, S. Creager, C. Creutz, Ch. Kagan, M. Kaneko, I. Okura (Eds.), Photocatalysis Science and Technology, P.V. Kamat, M. Lieberman, S. Lindsay, R. Marcus, R. Metzger, M.M. Kodasha-Springer, Tokyo, 2002. Beyerle, J. Miller, M. Newton, D. Rolison, O. Sankey, K. Schanze, G. Rincon, C. Pulgarin, Appl. Catal. B 49 (2004) 99–112. J. Yardley, X. Zhu, J. Phys. Chem. B 107 (2003) 6668–6697. R. Wang, K. Hashimoto, A. Fujishima, M. Cjikuni, E. Kojima, A.  A.Ya. Sychev, V.G. Isak, Russ. Chem. Rev. 64 (1995) 1105–1129. Kitamura, M. Shimohigoshi, Nature 388 (1997) 431.  T. Kornovalova, J. Lawrence, L. Kispert, J. Photochem. Photobiol. A. Matsuda, Y. Kotani, T. Kogure, M. Tatsumisago, T. Minami, J. A: Chem. 162 (2004) 1–8. Am. Ceram. Soc. 83 (2000) 229–231.  J. Pan, G. Benk¨ , Y. Xu, T. Pascher, L. Sun, V. Sundstr¨ m, T. o o H. Imai, H. Hirashima, J. Am. Ceram. Soc. 82 (1999) 2301–2304. Pol´vka, J. Am. Chem. Soc. 124 (2002) 13949–13950. ı